Optium Museum Acrylic

== Description ==
(Tru Vue®) Extruded acrylic sheet composed of a UV-blocking polymethyl methacrylate substrate with double-sided anti-reflective and anti-static coatings. It has been in use since at least 2004.
Acrylic glazing is chosen over glass for conservation purposes due to its shatter-resistance, light weight, and ease of machining. Optium Museum Acrylic is chosen over other types of acrylic sheets based on its proprietary coatings that impart high UV protection, anti-reflective and anti-static properties, and improved hardness that resists incidental marring.
== Applications ==
Optium Museum Acrylic is produced for use as glazing within frames and can be joined to create seamed flat panelsSmallCorp: Acrylic Glazing and Oversize Optium as well as three-dimensional vitrines and display cases. 
Though acrylic sheet such as Optium Museum Acrylic is commonly and effectively used for traveling displays, it should not be used in hermetically sealed cases, as acrylic is an inadequate barrier to water vapor.Phibbs, Hugh. 2014. Glass or Acrylic? Considerations for Framed Artwork.
Pressure-mounts for textiles often use lightweight and shatter-resistant acrylic glazing.Vuori, Jan, Renée Dancause & Stefan Michalski. 2017. Renewing the Past: Pressure Mounting a Large and Severely Fragmented Silk Flag, Journal of the American Institute for Conservation, 56:1, 59-74, DOI: 10.1080/01971360.2017.1287496 Testing on Optium Museum Acrylic has determined that the coatings are inert and thus the glazing is safe for direct contact with collection items.Williams, R. S., and J. Sirois. 2011. Optium Museum Acrylic Glazing. Report No. CSD 4873, CCI 100020. Canadian Conservation Institute, Ottawa.
The TruVue website has a large portfolio of projects which have used Optium Acrylic Glazing for object display cases, large-scale charcoal on paper, wall niches, framed tapestry, Japanese screens, climate-controlled packages for chalk on paper, library cabinet doors, and more.
== Personal Risks ==
While the product has been deemed non-hazardous, fabricators are advised to wear eye protection when cutting the acrylic sheet.
The acrylic base is a combustible thermoplastic, so caution should be taken around flames and sources of high heat.TruVue Case Fabrication Guidelines (English)
== Collection Risks ==
Links to Oddy Test results posted on AIC Wiki Materials Database Pages for individual materials below
*Optium Museum Acrylic: Tested in 2018, accessed 07/2020
== Environmental Risks ==
Acrylic resins are not commonly recycled. PMMA can be extracted at high purity from acrylic mixtures but only with the use of lead, complicating any positive environmental impact.AZO Materials. 2012. How Do You Recycle Acrylic Resin?
== Physical and Chemical Properties ==
Technical specifications from TruVueTruVue Optium Museum Acrylic
Substrate: 	Abrasion Resistant UV Filter Acrylic
Coating: 	Double-Sided Anti-Reflective
Reflection: 	<1.6% (double sided)
Transmission:	>98% (total)
UV Block: 	up to 99% of 300nm to 380nm UV rays
Avoid high temperatures. Acrylic sheet auto-ignites at 445°C/833°F and softens at 99°C/210°F.Optium Museum Acrylic SDS 
The polymethyl methacrylate of the acrylic sheet is soluble in esters, ketones, aromatic and chlorinated hydrocarbons.CAMEO: polymethyl methacrylate
== Working Properties ==
Sheets of Optium Museum Acrylic can be scored and snapped as long as they are 3.0mm or 4.5mm thick.TruVue FAQ: Cleaning, Cutting, and Handling Sheets of 6mm thickness must be cut with a saw, as laser cutting can disrupt the coatings. TruVue recommends an H-Series panel saw with a Plex-Cut PC860 saw blade from Everlast.TruVue Saw Blade Recommendations 
Heat-based fabrication methods like flame polishing, line bending, or thermo-forming will harm the coating and are not advised.
Miter joints are recommended for assembling 3-D structures, as butt joints require the removal of the coating on the uncut sheet so that the adhesive doesn't mar it.
TruVue recommends the following adhesives: Acrifix 2R1074 Vitrine (Evonik Industries), Weld-on 40 (IPS), PS-30 (Caseway Industrial Products), or Acrifix 192 (Evonik Industries).
This section's information and further details on coating removal, annealing, and edge polishing are available within the Case Fabrication Guidelines document.
== Forms and Sizes ==
Information from the TruVue Acrylic Collection Fact Sheet
Thickness 	Maximum Size 	Sq. Feet/Sheet 	Approx. Weight/Sheet
6.0mm (¼") 	72" x 120" (3048mm x 1829mm)	60 sq. ft (5.57 sqm)	89 lbs/40.37kg 1.5 lbs per ft² 7.2kg per m²
4.5mm (3/16")	72" x 96" (2438mm x 1829mm) 	48 sq. ft (4.46 sqm)	54 lbs/24.5kg 1.13 lbs per ft² 5.5kg per m²
3.0mm (⅛") 	48" x 96" (2438mm x 1219mm) 	32 sq. ft (2.97 sqm)	22 lbs/9.98kg 0.7 lbs per ft² 3.2kg per m²
Sizes available in 3mm sheets	16" x 20"	20" x 24"	24" x 32"	32" x 40"	36" x 48"	40" x 60"	48" x 96"
== Resources and Citations ==
*Kate Aguirre, contributed information, MWG group, 2020.
Category:Materials databaseCategory:MWGCategory:GlazingCategory: Board/Panel, Plastic